- Research article
- Open Access
In-vitro/In-vivo comparison of leuprolide acetate release from an in-situ forming plga system
© Mashayekhi et al.; licensee BioMed Central Ltd. 2013
- Received: 19 June 2012
- Accepted: 11 June 2013
- Published: 15 July 2013
A poly (lactide-co-glycolide) (PLGA) implant was used to control the release profile of leuprolide acetate (LA) drug. The system is an in-situ polymeric precipitation system. And the formulation consisted of PLGA polymer, LA drug and N-methyl-2-pyrrolidon solvent with no additives. First, the formulation was injected into PBS solution for in-vitro studies and then it was administered to the animal models (female rats) for in-vivo release studies. The release profiles of leuprolide acetate were measured by UV spectrophotometry for a period of 28 days. The initial burst release of LA was 14% in in-vitro whereas it was 7% in in-vivo. In-vitro and in-vivo release profiles of LA had similar trends after 72 hours. However, the rate of LA release was slower in-vivo. This might be attributed to the limited diffusion process of solvent and the drug molecules. This could be due to presence of an additional pressure caused by the surrounding tissue and also the presence of small amount of water between cells in the subcutaneous site. Cross-section and surface of the implants were studied via scanning electron microscopy. Morphology of both in-vitro and in-vivo implants confirmed the release behaviours. No toxicity effects were reported in the histopathological assay. Furthermore, the pharmacological analysis showed more inactive ovaries due to release of LA.
- Drug delivery system
- Biodegradable polymer
- Poly (lactide-co-glycolide) (PLGA)
An injectable in-situ polymeric system forms a solid or semisolid drug reservoir upon the parenteral injection of a drug solution. This is due to the permeation of water molecules into the implant, solvent removal process and coagulation of the polymer after injection[2, 3]. These systems have many advantages such as; ease of administration, having less complicated fabrication, increasing effective pharmacological duration, preserving the effectiveness of short lifetime drugs and reducing the need for repeated daily injection. However, they suffer from one major disadvantage, which is their high burst release defined as the amount of drug released during the first 24 hours[4, 5]. An undesirable high burst release may exhaust the loaded drug from the implants too rapidly and cause severe toxicity problems. It can also lead to an overall shorter drug release duration, and subsequently less therapeutic efficiency and cost-effectiveness.
Leuprolide acetate has been utilised for the treatment of the various diseases such as: advanced prostate cancer, breast cancer, uterine fibroids, endometriosis, and Alzheimer. LA is a synthetic analog of endogenous Gn-RH agonist and a non-apeptide drug. It increases the circulating levels of the luteinizing hormone (LH) and follicle-stimulating hormone (FSH) leading to a transient increase of gonadal steroids. In females, continuous administration of LA reduces the level of LH and FSH. But in males, the level of the testosterone increases right after the initial drug administration and then falls below the castrate threshold for the next 2–4 weeks. LA can be administered via parenteral and pulmonary routes[7, 8]. And it can be incorporated in different types of drug carriers such as nano/micro particles, capsules and in-situ forming implants. For instance, LA was successfully loaded in PLGA/PLA microspheres as an osmotical driven implantable system[9, 10].
PLGA is a FDA approved biodegradable alpha polyester. It has been used in several therapeutic applications and can be utilised in various forms of controlled release devices. For instances, it has been used as a suture mesh for a guidance around nerve defects, as a scaffold for cell proliferation and as drug delivery carriers with various forms. Moreover, N-methyl-2-pyrrolidone (NMP) is a water-soluble, water-miscible, biocompatible, and inert organic solvent with low toxicity potential in animal and human studies.
The main objective of this study is to investigate the release profile of leuprolide acetate from a PLGA injectable implant using in-vitro and in-vivo studies. PLGA implants were prepared and were injected into phosphate buffer saline (PBS) solution for the in-vitro studies. Subsequently, the same formulations were administered subcutaneously to the rat animal model for in-vivo studies. Drug release profiles were characterised using UV spectroscopy method. Structure and morphology of the PLGA implants were investigated in-vitro and in-vivo via scanning electron microscopy. The toxicity effects of the implants on the living tissues were investigated by a histopathological assay on sexual and non-sexual organs. Furthermore, the pharmacological analysis was conducted to study the influence of the LA release on the ovaries and the uterine of the animal models within 28 days.
Poly (lactide-co-glycolide) (50:50), Resomer® RG 504, (Mw=48,000 Da) as a biodegradable copolymer, was obtained from Boehringer Inc. (Ingelheim, Germany) for sterilization. Leuprolide acetate (Mw 1209 Da) was supplied by Bachem Inc. (Bubendorf, Switzerland). Analytical grade N-methyl-2-pyrrolidon was purchased from Merck (Riedel-deHaen Company, German).
The RG 504 PLGA polymer and NMP as a solvent were used. First, the polymer was mixed with NMP in the specific ratio of PLGA (28 wt %) to NMP (69 wt %) by a glass mixer. Subsequently, the mixture was placed on a continuous shaker in order to obtain clear solutions after 1 hour. The PLGA solutions were gamma irradiated (dose of 25kGy). Then 3 wt % leuprolide acetate was dissolved in the polymer solution. The sample preparation was performed at ambient temperature (23°C ± 3°C).
0.5 g of the formulations were injected into 15 ml PBS (0.2 M, pH 7.4) through a 20 gauge needle and were stored at 37°C in an incubator. 15 ml PBS released media was taken and replaced at the determined time points (0, 1, 2, 3, 7, 14, 18, 21, 25, 28 days). The concentration of the leuprolide acetate was calculated by UV spectrophotometer.
Female Sprauge-Dawley rats (8 weeks old, 150±5 g) were used. The formulation was injected subcutaneously on the back using 16 gauge needle. The animal models were divided into 3 groups (Group A, B and C). Group A (n=21) were administered with 100 (μg/kg/day) of LA, and Group B (n=21), received the formulation without drug 10 (μg/kg/day) of formulation. Group C (n=3) was the control group and they were sacrificed in the first day. This point is important that the research on animals was acted in pathology department in "Iran Veterinary Organization" with ethical approval (ISO 17025) from TUV (Germany).
Determination of leuprolide acetate (LA)
UV spectrophotometer (CECIL 1000 SERIES, England) was used for in-vitro and in-vivo release studies. In in-vitro release studies, the amounts of drug released in PBS were measured at discrete time intervals. For in-vivo release studies, the remainder PLGA implants were first dissolved in 10 ml NMP. Then, the amounts of the leuprolide acetate in the implants were calculated. Samples without LA were also monitored so that any contributions to the measured absorbance from the polymer could be evaluated.
The UV-spectroscopy method was carried out at wavelength of 279 nm. The developed method was validated with respect to linearity, accuracy (recovery), precision and specificity in accordance with ICH (International Conference on Harmonisation) requirements for assay method determination.
Specificity was investigated by determining the blank dissolution media and the dissolution media containing LA and any other potential excipients by UV, then spiking the drug substance and examining any interference between peaks. To determine the linearity and range of the assay method, standard solutions of LA having known concentrations were used; these standards have been analysed with the UV method as described. For each concentration, 3 runs have been performed. Accuracy was evaluated by analysing synthetic mixtures spiked with known quantities of drugs. Linearity was studied in the range of 1–25 μg/ml of the analyte content. The calibration curve obtained had a R2 value of 0.998, an intercept of 0.004 and a slope of 0.007; the intervals at 95% confidence level, calculated for the intercept included the zero value. Accuracy was determined at three levels of content in placebo. Recovery ranged from 98 to 103.5 with a mean value of 101.3 a RSD % of 0.85 and finally in the specificity term we have not seen any interference between API and other excipients. Thus the method showed an acceptable degree of linearity, accuracy and precision according to the validation requirements and can be considered valid.
Scanning electron microscopy (SEM)
The surface morphologies and the cross-sections of the PLGA implants were studies by SEM (Cambridge S360, England) at predetermined times (24 h, 3, 7, and 14 days). Samples were frozen and mounted on metal stubs with double-sided carbon tape and coated with gold (30 mA for 5 min) by a sputter coater (E 5200 AUTO, BioRAD Polaron Devision, England). The morphologies of the in-vivo samples after the day 14 were not studied because of significant degradation of the implants.
Pharmacological and histopathological analysis
The animal models were scarified at the defined time points. Their non-sexual organs (lung, liver, kidney) and sexual organs (four layers of uterine and ovaries) were fixed with 10% neutralised formalin. The paraffin method was utilised for preparation of paraffin blocks and sections were cut and mounted on microscope slides. The sections were stained by hematocyline and eosin for histological investigation and these were studied using a light microscope.
The in-vivo and in-vitro release data were analysed statistically, with ANOVA using Minitab 14.
PLGA degrades by means of hydrolysis including surface hydrolysis, bulk hydrolysis, and bulk catalysed hydrolysis. The inwards diffusion of the aqueous phase causes degradation of the polymer chains which in turn facilitates the diffusion of the entrapped drug. The biodegradation products of PLGA (lactic and glycolic acid) are common body metabolites, which are non-toxic, non-immunogenic, non-carcinogenic, and non-teratogenic. However, the products of polymer degradation can be trapped in the internal structure, which can change the localised pH within the polymer matrix. This phenomenon accelerates the polymer degradation due to autocatalysis.
Furthermore, PLGA erosion was determined by monitoring the pH changes and lactic acid formation as a reaction of the degradation. There was a lag-phase in formation of lactic acid in the first 4 days. The pH of the release medium was 7 and the drug release rate was not noticeable at this stage. The pH of the environment decreased afterward due to the degradation of the PLGA implant and the presence of lactic acid in the release medium.
In this study, the mechanism of the LA release had 4 stages: (i) diffusion of drug through the polymer; (ii) surface erosion of the polymer and continuous release of the physically entrapped drug; (iii) cleavage of the covalent bonds between the polymer bulks followed by the drug diffusion; and (iv) slow diffusion of LA through the polymer and degradation of the polymer until drug depletion.
The morphology and structure of a blank PLGA implant (with no drug) was also studied. The SEM micrographs were similar to the SEM micrographs of the implant loaded with LA in terms of the degree of their porosities and their internal structures. These similarities were observed throughout the 28 days of the studies, except from day 3. The surface of the implant had much less pores during this period in the blank implant.
All implants used in human body should be biocompatible and non-toxic. In this study, it was observed that all tissue samples had normal structures with no necrotic tissues. And the implant does not possess any toxicity effects on the living tissues and organs including the tissues at the injection site and sexual/non-sexual organs.
Comparison of in-vitro and in-vivo results
The amount of leuprolide acetate released in in-vitro and in-vivo environments
The release profiles of LA from injectable in-situ forming PLGA implants were studied in in-vitro and in-vivo environments. The release profiles had four phases in the in-vitro study. It started with a burst release phase where 14% of the loaded drug was released in the first 24 hours. The rate of the drug release in the initial phase was lower in the in-vivo environment and the amount of release drug was only 8% in the first 24 hours. However, the release profiles had similar trends after day 3 in both in-vitro and in-vivo environments. Histopathology studies confirmed that the implants were biocompatible and no toxicity effects were observed on the various living tissues and organs. Pharmacology studies revealed that the LA loaded implants were effective in suppressing the gonadotropin receptors and halting the ovaries function.
- Hammer KS, Boisclair J, Schuetz H, Petersen H, Goepferich A: Biocompatibility of an Injectable in-situ Forming Depot for Peptide Delivery. Pharm. Sci. 2010, 99: 4390-4399. 10.1002/jps.22149.View ArticleGoogle Scholar
- Fogueri LR, Singh S: Smart Polymers for Controlled Delivery of Proteins and Peptides. A Review of Patents. 2009, 3 (7): 40-48.Google Scholar
- Kranz H, Brazeau GA, Napaporn J, Martin RL, Millard W, Bodmeier R: Myotoxicity studies of injectable biodegradable in-situ forming drug delivery system. Int J Pharm. 2001, 212: 11-10.1016/S0378-5173(00)00568-8.View ArticlePubMedGoogle Scholar
- Bodmeier S, López Esguerra V, Körber M, Dong WY: Stability of poly (D,L-lactide-co-glycolide) and leuprolide acetate in in-situ forming drug delivery systems. J.C.R. 2006, 115 (2): 158-167. 10.1016/j.jconrel.2006.07.013.View ArticleGoogle Scholar
- Dunn RL, Garrett JS, Ravivarapu H, Chandrashekar BL: Polymeric delivery formulations of Leuprolide with improved efficacy. US Patent. 2004, 6: 773,714-Google Scholar
- Okada H, Doken Y, Ogawa Y: Persistent Suppression of the Pituitary-Gonadal System in Female Rats by Three-Month Depot Injectable Microspheres of Leuprorelin Acetate. J Pharm Sci. 1996, 85 (10): 1045-View ArticleGoogle Scholar
- Hatano T: Incidence of bone fracture in patients receiving luteinizing hormone-releasing hormone agonists for prostate cancer. BJU Int. 2000, 86: 449-452. 10.1046/j.1464-410X.2000.00774.x.View ArticlePubMedGoogle Scholar
- Eligard SO: leuprolide acetate in a novel sustained-release delivery system. Urology. 2003, 61 (2Suppl 1): 25-31.Google Scholar
- Bari H: Inter A, prolonged release parenteral drug delivery system. Inter. J Pharm. Sci. Rev. Res. 2010, 3 (1): 1-11.Google Scholar
- Zare M, Mobedi H, Barzin J, Mivehchi H, Jamshidi A, Mashayekhi R: Effect of Additives on Release Profile of Leuprolide Acetate in an In-situ Forming Controlled-Release System: In-vitro Study. J. Appl. Poly. Sci. 2008, 107: 3781-3787. 10.1002/app.27520.View ArticleGoogle Scholar
- Krogman NR, Singh A, Nair LS, Laurencin CT: Allcock HR. Biomacromolecules. 2007, 8: 13106-13125.View ArticleGoogle Scholar
- Dunn RL, Garrett JS, Ravivarapu H, Chandrashekar B: Polymeric delivery formulations of leuprolide with improved efficacy. US Patent. 2003, 656: 5874-Google Scholar
- Strickley RG: Solubilizing excipients in oral and injectable formulations. Pharm Res. 2001, 21: 201-230.View ArticleGoogle Scholar
- Okada H, Inoue Y, Heya T, Ueno H, Ogawa Y, Toguchi H: Pharmacokinetics of once-month injectable microspheres of leuprolide acetate. Pharm Res. 1991, 8 (6): 787-791. 10.1023/A:1015818504906.View ArticlePubMedGoogle Scholar
- Guideline, I.C.H.H.T:Validation of analytical procedures: Methodology. ICH. 1996,Google Scholar
- Luan X, Bodmeier R: Influence of the poly (lactide-co-glycolide) type on the Leuprolide release from in-situ forming microparticle systems. J.C.R. 2006, 110: 266-272. 10.1016/j.jconrel.2005.10.005.View ArticleGoogle Scholar
- Bakhshi R, Vasheghani-Farahani E, Mobedi H, Jamshidi A, Khakpour M: The effect of additives on naltrexone hydrochloride release and solvent removal rate from an injectable in-situ forming PLGA implant. Poly. Adv. Tech. 2006, 17: 354-359. 10.1002/pat.717.View ArticleGoogle Scholar
- Luan X, Bodmeier R: Modification of the tri-phasic release pattern of Leuprolide Acetate-loaded poly (lactide-co-glycolide) microparticles. Euro. J. Pharm. Biopharm. 2006, 63: 205-214. 10.1016/j.ejpb.2005.12.010.View ArticleGoogle Scholar
- Khang G, Kyuang JE, Rhee JM: Controlled release of nerve growth factor from sandwiched poly (D, L-lactide-co-glycolide) films for the application in neural tissue engineering. Macromol Res. 2003, 11 (5): 334-340. 10.1007/BF03218373.View ArticleGoogle Scholar
- Astaneh R, Moghimi HR, Erfan M, Mobedi H: Formulation of an injectable implant for peptide delivery and mechanistic study of the effect of polymer molecular weight on its release behavior. DARU. 2006, 14 (2): 65-70.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.